Unknown quantum electronic conductance across nanojunctions made of silicon-doped carbon wires between carbon leads is investigated. This is done by an appropriate generalization of the phase field matching theory for the multi-scattering processes of electronic excitations at the nanojunction and the use of the tight-binding method. Our calculations of the electronic band structures for carbon, silicon, and diatomic silicon carbide are matched with the available corresponding density functional theory results to optimize the required tight-binding parameters. Silicon and carbon atoms are treated on the same footing by characterizing each with their corresponding orbitals. Several types of nanojunctions are analyzed to sample their behavior under different atomic configurations. We calculate for each nanojunction the individual contributions to the quantum conductance for the propagating σ, Π, and σ∗electron incidents from the carbon leads. The calculated results show a number of remarkable features, which include the influence of the ordered periodic configurations of silicon-carbon pairs and the suppression of quantum conductance due to minimum substitutional disorder and artificially organized symmetry on these nanojunctions. Our results also demonstrate that the phase field matching theory is an efficient tool to treat the quantum conductance of complex molecular nanojunctions.
Quantitative analysis of electronic quantum transport in nanostructures is essential for the development of nanoelectronic devices . The monatomic linear carbon wire (MLCW) systems are expected in this context to have potentially interesting technological applications, in particular as connecting junction elements between larger device components . In this respect, electronic quantum transport properties are the key features of such wire nanojunctions .
Carbon exists in nature under a wide range of allotropic forms as the two-dimensional graphene , the cage fullerenes , and the quasi one-dimensional carbon nanotubes . These forms exhibit exceptional physical properties and can be considered as promising components for future nanodevices . The discovery of MLCW, [8–14] turns the attention to another intriguing carbon allotropic form. In the experiment conducted recently by Jin et al. , MLCW was produced by directly removing carbon atoms row by row from the graphene sheets, leading to a relatively stable freestanding nanostructure.
At present, the available experimental data do not provide essential knowledge about the electronic properties of MLCW systems, and only theoretical studies shed some light on these properties. Furthermore, although the MLCW systems were investigated for a long time from the theoretical point of view [15–26], their interest was not highlighted until recently due to the open attention paid to other carbon allotropic forms. It has been shown in particular that from the structural point of view, MLCW can form either as cumulene wires (interatomic double bonds) or polyyne wires (alternating interatomic single and triple bonds) [14, 17, 19, 27, 28]. However, there is no straightforward answer as to which of these two structures is the favorable one; experimental studies do not give a satisfactory answer, and theoretical calculations yield provisions which depend on applied computational methods. Density functional theory (DFT) calculations predict double-bond structures [29, 30], whereas ab initio Hartree-Fock (HF) results favor alternating bond systems [15–18, 27]. This situation arises from the fact that DFT tends to underestimate bond alternation (second-order Jahn-Teller effect), while HF overestimates it .
More recently, first-principle calculations have indicated  that both structures are stable and present mechanical characteristics of a purely one-dimensional nanomaterial. Moreover, on the basis of the first-principle calculations [31–42], the cumulene MLCW wires are expected to be almost perfect conductors, even better than linear gold wires , while the corresponding polyyne wires are semiconducting . It is also worth noting that the MLCW cumulene system may exhibit conductance oscillations with the even and odd numbers of the wire atoms [28, 42].
In the present work, we consider in particular the problem of the electronic quantum transport across molecular nanojunctions made up of silicon-doped carbon wires, prepared in ordered or substitutionally disordered configurations as in the schematic representation of Figure 1, where the nanojunctions are between pure MLCW wire leads. This problem has not been considered previously and is still unsolved to our knowledge. The interest in the quantum transport of such nanojunctions arises from the fact that chemical defects or substitutional disorder may have a significant impact on their transport properties . Chemical impurities doping the nanojunction may even allow the control of the transport for such nanostructures . The properties of the nanoelectronic device and its functionality may hence be greatly affected or even built on such ordered and disordered configurations. The interest in silicon carbide, furthermore, stems from the fact that it is considered a good substrate material for the growth of graphene  and may produce interesting effects in its interactions with Si or C .
The electrons which contribute to transport present characteristic wavelengths comparable to the size of molecular nanojunctions, leading to quantum coherent effects. The transport properties of a given nanojunction are then described in terms of the Landauer-Büttiker theory [47, 48], which relates transmission scattering to quantum conductance. Several approaches have been developed in order to calculate the scattering transmission and reflection cross sections in nanostructures, where the most popular are based on first-principle calculations [49, 50] and semiempirical methods using the non-equilibrium Green’s function formalism [51, 52].
In the present work, we investigate the electronic scattering processes on the basis of phase field matching theory (PFMT) [53, 54], originally developed for the scattering of phonons and magnons in nanostructures [55–59]. Our theoretical method is based on appropriate phase matching of the Bloch states of ideal leads to the local states in the scattering region. In this approach, the electronic properties of the system are described in the framework of the tight-binding formalism (TB) which is widely exploited for electronic transport calculations [54, 60–63] and for simulating the STM images of nanostructures [64, 65]. In particular, we employ the appropriate Slater-Koster  type Hamiltonian parameters calculated on the basis of the Harrison’s tight-binding theory (HTBT) . The PFMT method, which is formally equivalent to the method of non-equilibrium Green’s functions , can be considered consequently as a transparent and efficient mathematical tool for the calculation of the electronic quantum transport properties for a wide range of molecular-sized nanojunction systems.
The present paper is organized in the following manner. In the ‘Methods’ section, we give the detailed discussion of theoretical PFMT formalism. Our numerical results, which incorporate propagating and evanescent electronic states, are presented per individual lead modes in the ‘Results and discussion’ section. Also presented are the total conductance spectra; they are compared with results based on first-principle calculations when available. Finally, the discussion and conclusions are given in the ‘Conclusions’ section. Appropriate appendices which supplement the theoretical model are also presented.
Theoretical model and propagating states
The schematic representation of the system under study with an arbitrary nanojunction region is presented in Figure 1. With reference to the Landauer-Büttiker theory for the analysis of the electronic scattering processes [47, 48], this system is divided into three main parts, namely the finite silicon-doped carbon wire nanojunction region, made up of a given composition of carbon (black) and silicon (orange) atoms, and two other regions to the right and left of the nanojunction which are semi-infinite quasi one-dimensional carbon leads. Moreover, for the purpose of quantum conductance calculations, the so-called irreducible region and the matching domains are depicted (see the ‘Phase field matching theory’ subsection for more details). Figure 1 is used throughout the ‘Methods’ section as a graphical reference for analytical discussion.
The system presented in Figure 1 is described by the general tight-binding Hamiltonian block matrix:
This is defined in general for a system of N x inequivalent atoms per unit cell, where N l denotes the number of basis orbitals per atomic site, assuming spin degeneracy. In Equation 1, Ei,j denotes on-diagonal matrices composed of both diagonal and off-diagonal elements for a selected unit cell. In contrast, the Hi,jmatrices contain only off-diagonal elements for interactions between different unit cells. The index α identifies the atom type, C or Si, on the n th site in a unit cell. Each diagonal element is characterized by the lower index l for the angular momentum state. The off-diagonal elements describe the m-type bond, (m=σ,Π), between l and l′ nearest-neighbor states. The index β identifies the types of interacting neighbors, C-C, Si-Si, or Si-C.
where values are the dimensionless Harrison coefficients; m e , the electron mass in vacuum; and d β , the interatomic distance for interacting neighbors. Explicit forms of the Ei,j and Hi,j matrices are given in Appendix Appendix 1. The tight-binding parameter schemes are illustrated in Figure 1; however, it is noteworthy that the n and n′indices for coupling parameters are dropped for simplicity in this figure.
In our calculations, the single-particle electronic wave functions are expanded in the orthonormal basis of local atomic wave functions ϕ l (r) as follows:
In Equation 3, k is the real wave vector; R N , the position vector of the selected unit cell; and R N , the position vector of the n th atom in the selected unit cell. For ideal leads, the wave function coefficients c l (r n −R N ,k) are characterized under the Bloch-Floquet theorem in consecutive unit cells by the following phase relation:
where z is the phase factor
which corresponds here to waves propagating to the right (+) or to the left (−).
The electronic equations of motion for a leads unit cell, independent of N, may be expressed in a square matrix form, with an orthonormal minimal basis set of local wave functions as follows:
E stands for the electron eigenvalues, and I is the identity matrix, while the dynamical matrix M d contains the Hamiltonian matrix elements and the z phase factors; c(k,E) is the N x ×N l size vector defined as follows:
Equation 6 gives the N x ×N l eigenvalues with corresponding eigenvectors which determine the electronic structure of the lead system, where l under the vector c l corresponds to N l =4 orbitals s,p x ,p y ,p z . Note that the choice of an orthonormal minimal basis set of local wavefunctions may result initially in an inadequate description of the considered electronic eigenvalues. However, as can be seen later, the proper choice of the TB on-site energies and coupling terms allows us to to obtain agreement with the DFT results. This is a systematic procedure in our calculations.
The complete description of electronic states on the ideal leads requires a full understanding of the propagating and evanescent electronic states on the leads. This arises because the silicon-doped nanojunction breaks the perfect periodicity of the infinite leads and forbids a formulation of the problem only in terms of the pure Bloch states as given in Equation 5. Depending on the complexity of a given electronic state, it follows that the evanescent waves may be defined by the phase factors for a purely imaginary wave vectors k=i κ such that
or for complex wave vectors k=κ1 + i κ2such that
The phase factors of Equations 8 and 9 correspond to pairs of hermitian evanescent and divergent solutions on the leads. Only the evanescent states are physically considered where spatial evanescence occurs to the right and left, away from the nanojunction localized states. It is important to note that the l-type evanescent state corresponds to energies beyond the propagating band structure for this state.
The functional behavior of z(E) for the propagating and evanescent states on the leads may be obtained by various techniques. An elegant method presented previously for phonon and magnon excitations  is adapted here for the electrons. It is described on the basis of Equations 4 and 6 by the generalized eigenvalue problem for z:
Equation 10 gives the 2N x N l eigenvalues as an ensemble of N x N l pairs of z and z−1. Only solutions with |z|=1 (propagating waves) and |z|<1 (evanescent waves) are retained as physical ones. In Equation 10, k is then replaced by the appropriate energy E variable. Furthermore, for systems with more than one atom per unit cell, the matrices HN,N−1 and in this procedure are singular. In order to obtain the physical solutions, the eigenvalue problem of Equation 10 is reduced from the 2N x N l size problem to the appropriate 2N l one, using the partitioning technique (please see Appendix Appendix 2).
Phase field matching theory
The scattering problem at the nanojunction is considered next. An electron incident along the leads has a given energy E and wave vector k, where E=E γ (k) denotes the available dispersion curves for γ = 1, 2,.., γ propagating eigenmodes, where γ corresponds to the total number of allowed solutions for the eigenvalue problem of phase factors in Equation 10. In any given energy interval, however, these may be evanescent or propagating eigenmodes and together constitute a complete set of available channels necessary for the scattering analysis.
The irreducible domain of atomic sites for the scattering problem includes the nanojunction domain itself, (N∈[0,D−1]), and the atomic sites on the left and right leads which interact with the nanojunction, as in Figure 1. This constitutes a necessary and sufficient region for our considerations, i.e., any supplementary atoms from the leads included in the calculations do not change the final results. The scattering at the boundary yields then the coherent reflected and transmitted fields, and in order to calculate these, we establish the system of equations of motion for the atomic sites (N∈[−1,D]) of the irreducible nanojunction domain.
This procedure leads to the following general matrix equation:
M nano is a (D + 2)×(D + 4) matrix composed of the block matrices , and the state vector V of dimension D + 4 is given as follows:
Since the number of unknown coefficients in Equation 11 is always greater than the number of equations, such a set of equations cannot be solved directly.
Assuming that the incoming electron wave propagates from left to right in the eigenmode γ over the interval of energies E=E γ , the field coefficients on the left and right sides of the irreducible nanojunction domain may be written as follows:
where γ′∈Γ is an arbitrary channel into which the incident electron wave scatters, and c l (r n ,z γ ,E γ ) denotes the the eigenvector of the lead dynamical matrix of Equation 6 for the inequivalent site n at z γ and E γ . The terms and denote the scattering amplitudes for backscattering and transmission, respectively, from the γ into the γ′eigenmodes and constitute the basis of the Hilbert space which describes the reflection and transmission processes.
Equations 13 and 14 are next used to transform the (D + 2)×(D + 4) matrix of the system of equations of motion, Equation 11, into an inhomogeneous (D + 2)×(D + 2) matrix for the scattering problem. This procedure leads to the new form of the following vector:
The rectangular sparse matrix in Equation 15 has the (D + 4)×(D + 2) size. The vectors and are column vectors of the backscattering and transmission Hilbert basis.
In Equation 16, M is the matched(D + 2)×(D + 2) square matrix, and the vector of dimension (D + 2) which incorporates the and elements, regroups the inhomogeneous terms of the incident wave. The explicit forms of the M matrix elements and and vectors are presented in Appendix Appendix 3.
In practice, Equation 16 can be solved using standard numerical procedures, over the entire range of available electronic energies, yielding the coefficient c l for atomic sites on the nanojunction domain itself as well as the γ reflection and the γ transmission coefficients.
The reflection and transmission coefficients give the reflection and transmission probabilities, respectively, by normalizing with respect to their group velocities v γ in order to obtain the unitarity of the scattering matrix as follows:
where v γ ≡v γ (E) denotes the group velocity of the incident electron wave in the eigenmode γ. The group velocities are calculated by a straightforward procedure as in Appendix Appendix 4. For evanescent eigenmodes, . Although the evanescent eigenmodes do not contribute to the electronic transport, they are required for the complete description of the scattering processes.
Furthermore, using Equations 17 and 18, the overall reflection probability, R γ (E), for an electron incident in the γ eigenmode and the total electronic reflection probability, R(E), from all the eigenmodes may be expressed, respectively, as follows:
Similarly, for transmission probabilities, we may write the equivalent equations as follows:
The T γ (E) and T(E) probabilities are very important for the electronic scattering processes since they correspond directly to the experimentally measurable observables. Likewise, the total transmission T(E γ ) allows to calculate the overall electronic conductance. In this work, we assume the zero-bias limit and write the total conductance in the following way:
In Equation 21, G0 is the conductance quantum and equals 2e2/h. Due to the Fermi-Dirac distribution, G(E F ) is calculated at the Fermi level of the perfect lead band structure since electrons only at this level give the important contribution to the electronic conductance. The Fermi energy can be determined using various methods where, in the present work, E F is calculated as the basis of the density of state calculations.
Results and discussion
The tight-binding model and basic electronic properties
In this section, we present the results of our model calculations for the electronic structure of carbon, silicon, and silicon carbide wires under study. Our results are validated by comparison with DFT calculations [29, 69], which allow us to establish unambiguously our choice of the tight-binding parameters for these systems.
In principle, we can develop our model calculations for the nanojunctions and their leads using any adequate type of orbitals; even a single orbital suffices to calculate the electronic quantum transport for carbon nanojunctions . However, this approximation is inadequate for silicon atoms. To treat both types of atoms on the same footing, we thus characterize the atoms by the electronic states 2s and 2p for carbon and by 3s and 3p for silicon. Such a scheme gives us four different orbitals, namely s, p x , p y , and p z , for both types of atoms.
In the present work, our TB parameters are effectively rescaled from the Harrison’s data in order to match our model calculations for the electronic structure with those given by the DFT. The utilized TB parameters are presented in Table 1 in comparison with the values given by Harrison. It is worthy to note that the values of the on-site Hamiltonian matrix elements are identical for states p x , p y , and p z . The off-diagonal distance-dependent elements are calculated on the basis of Equation 2. For symmetry considerations, these latter elements are positive or negative, also hs,p,σ = ηs,p,σ = 0 and hp,p,σ = ηp,p,σ = 0, for p y and p z , and . Table 1 is supplemented for the reader by Figure 2 which gives the dependence of the hopping integrals with distance as calculated in the present paper (continuous curves), in comparison with the Harrison’s data (open symbols).
Figure 2 clearly indicates the fact that qualitatively, both Harrison’s and our rescaled coupling parameters for silicon, carbon and diatomic silicon carbide wires, present the same functional behavior, confirming the desired conservation of their physical character. However, most of the rescaled coupling parameters have somehow smaller values than those initially proposed by Harrison; this trend can be also traced in Table 1 for the onsite parameters. This difference stems from the influence of the low-coordinated systems are considered here, whereas the initial Harrison values are given to match tetrahedral phases . Another general observation can be made for the tight-binding parameters of the σ-type interactions (the hs,p,σand hp,p,σones), which present much closer values over the considered interatomic distance range than in the case of Harrison’s data.
Our calculated electronic band structures for silicon, carbon, and diatomic silicon carbide infinite wires (continuous curves) are presented in Figure 3 in comparison with the DFT results [29, 69] as in the right-hand side of the figures. We note for the carbon and silicon structures that our TB parameters correctly reproduce the DFT results up to energies slightly above the Fermi level. Electronic branches in the regions of high energies are in qualitative agreement. In the case of the diatomic silicon carbide structure, some of the electronic states perfectly match the DFT results even for high-energy domains. The left-hand side of Figure 3 compares our results (continuous curves) with those from the older TB values given by Harrison (open symbols); as is seen, our TB parameters constitute the most optimal set for the electronic transport calculations since their corresponding electronic band structures conform to the appropriate energy ranges highlighted by the DFT results and, what is even more important, correctly reproduce the Fermi level.
In Figure 3A,B for silicon and carbon, the red and blue colors correspond, respectively, to the σ and σ∗ bands. These arise from the s p x orbital hybrids where the lowest lying bands are always occupied by two electrons. Bands marked by the red color have the Π character and are degenerate. Their origin in the p y and p z orbitals allows them to hold up to four electrons. In Figure 3C for the diatomic silicon carbide, starting from the band structure minimum, consecutive bands have their origin in the following orbitals: carbon 3s (red band), silicon 3s (green band), carbon 3p (blue and black bands), and silicon 3p (orange and violet bands). The blue and orange colors for the silicon carbide electronic structure indicate two doubly degenerate Π-type bands.
The metallic or insulating character of the considered atomic wires, following the Fermi level, is appropriate only when the wires are infinite. It is well known that this character can change for the case of finite size wires with a limited number of atoms or due to the type and quality of the leads.
Numerical characteristics for the carbon leads
In general, the infinite carbon wires which are considered as the leads in our work, present electronic band structure characteristics which incorporate not only propagating (see Figure 3A), but also evanescent states. Both of these types of states, which are derivable from the generalized eigenvalue problem as presented in Equation 10, constitute a complete set over the allowed energies for the electrons incident along the leads, which can be further scattered at the considered nanojunction. This complete set of eigenstates is used as the basis for the numerical calculations of the quantum conductance presented in the ‘Transport properties’ subsection.
Figure 4A presents the three-dimensional representation of the solutions of Equation 10 as a set of generalized functionals z(E) for the σ, σ∗, and Π electronic states of the carbon leads. As described by Equations 5, 8, and 9, the eigenstates in Figure 4A characterized by |z|=1 correspond to the propagating electronic waves described by the real wave vectors, whereas those by |z|<1 correspond to the evanescent and divergent eigenstates for the complex wave vectors. Furthermore, for convenience, the corresponding moduli of the complex z factors are presented in Figure 4B. Note that |z|=1 solutions may be grouped into pairs for the two directions of propagation linked by time-reversal symmetry. Due to the fact that each of these two solutions provides the same information, we consider waves propagating only from left to right. However, this is not true for the |z|<1 solutions which are always considered for both left and right as spatially evanescent. As can be seen in Figure 4, the generalized results for σ, σ∗, and Π states are represented by the same colors as the corresponding states in Figure 3A, following their propagating character for |z|=1, and further extended to the physically |z|<1 evanescent solutions.
Figure 4 provides a more complete description for the electronic states of a given system compared to a typical band structure representation as in Figure 3, since both the propagating and evanescent states are shown. Such a general representation clearly indicates the importance of the evanescent eigenstates for a full description of the scattering problem presented in the ‘Transport properties’ subsection. The energies considered in our calculations correspond to the range within the band structure boundaries, marked by two vertical dotted lines in Figure 4B. As a consequence, not only the propagating states, but also the evanescent solutions are included in the quantum conductance calculations in the ‘Transport properties’ subsection.
In this subsection, the electronic transport properties of nanojunction systems composed of silicon-doped carbon wires between carbon leads are calculated using the PFMT method. Figure 5A presents a number of these systems where we indicate the irreducible domains by the shaded grey areas. Note that these systems are always composed of finite nanojunction regions of silicon and carbon atoms, coupled with two carbon semi-infinite leads. The first three systems of Figure 5 correspond to periodic diatomic silicon carbide nanojunctions composed of 1, 2, and 3 Si-C atomic pairs, respectively. The next system corresponds to a nanojunction with a substitutional disorder, composed of three carbon and three silicon atoms. The last is a symmetric nanojunction of five silicon atoms and only one carbon atom in the middle. Figure 5B presents the group velocities of electrons in the carbon leads.
The calculated transmission and reflection scattering cross sections for each of the four available transport channels are presented in Figure 6. Each row of the figure corresponds to a nanojunction system (NS) as follows: Figure 6A,B,C for NS 1, Figure 6D,E,F for NS 2, Figure 6G,H,I for NS 3, Figure 6J,K,L for NS 4, and Figure 6M,N,O for NS 5. The red and green continuous curves represent the transmission and reflection spectra, respectively. The blue histograms correspond to the free electronic transport on the carbon leads, i.e., to the electronic transport on the perfect infinite quasi one-dimensional carbon wire over the different propagating states. These histograms constitute the reference to the unitarity condition which is used systematically as a check on the numerical results. The leads’ Fermi level is marked by a dashed line and set as a zero-energy reference. Under the zero-bias limit, the total conductance is calculated at this Fermi level.
In Figure 6, the transmission spectra present strong scattering resonances, showing an increasing complexity with the increasing size and configurational order of the nanojunctions. The valence σ state exhibits negligible transmission for all of the considered nanojunctions. The degenerate Π states and the σ∗state present in contrast the finite transmission spectra. However, it is only the Π states which cross the Fermi level, giving rise to electronic conductance across the nanojunction within the zero-bias limit.
In particular, the first three considered systems represent increasing lengths of the diatomic silicon carbide nanojunction with the increasing number of ordered Si-C atomic pairs. The transmission at the Fermi level for these systems is nonzero (see Figure 3C), which contrasts with the insulating character of the infinite silicon carbide wire. One can connect this finite transmission to the indirect bandgap (Δ) around the Fermi level for the diatomic silicon-carbide infinite wire (for more details, please see Figure 3C). This gap, Δ∼1. 5 eV, is indeed related to the difference between the binding energies of the silicon and carbon atoms and corresponds to an effective potential barrier for the propagating Π-state electrons. As the wire length increases by adding Si-C atomic pairs, as for systems 1 to 3 of Figure 5B, the transmission decreases due to cumulative barrier effects. We note that a similar effect for the monovalent diatomic copper-cobalt wire nanojunctions has been observed in a previous work .
Furthermore, it is instructive to compare the scattering spectra for the degenerate Π states, for nanojunction systems 3 and 4. These two systems contain identical numbers of silicon and carbon atoms; however, system 3 is an ordered configuration of Si-C pairs, whereas system 4 presents substitutional disorder of the atoms. It is seen that the disorder suppresses the conductance of the Π-state electrons at the Fermi level within the zero-bias limit. Another general observation can be made from the results for nanojunction system 5 which contains more silicon than carbon atoms. Despite the finite size of this system, which is comparable to system 4, and despite the structural symmetry of its atomic configuration, the electronic transmission is suppressed at the Fermi level within the zero-bias limit. This implies that one of the main observations of our paper is that structural symmetry on the nanojunction is not a guarantee for finite transmission in the case of the multivalence diatomic wire nanojunctions.
Figure 6 also shows that the transmission spectra for the σ∗ state are close to unity over a significant range of energies from approximately 1 to 7 eV for all of the five nanojunction systems. This result may prove useful for the electronic conductance across silicon-doped carbon nanojunctions under finite bias voltages.
In Figure 7, we present the total electronic conductance G(E) as a function of energy E and in units of G0=2e2/h for the considered nanojunction systems of a given length as depicted in Figure 5 (red). Moreover, the perfect electronic conductance on the carbon leads (blue) is given in comparison and constitutes effectively the conductance of the infinite and perfect quasi one-dimensional carbon wire. In Figure 7, the Fermi level is indicated by the dashed line as a zero-reference energy, and G(E) is calculated from all the contributing eigenstates of Figure 6, including the two degenerate Π states.
We note that the conclusions given for the results presented in Figure 6 are also followed by the more general representation of the electronic transport depicted in Figure 7. Furthermore, the results presented in Figure 7 confirm that only the electrons incident from the leads in the Π states are responsible for the electronic conductance at the zero-bias limit, which is readable from the Fermi level position. However, for all considered systems, the conductance at the Fermi level is theoretically limited to the value of 2 G0, and the biggest conductance maxima close to the perfect infinite carbon wire value of 3 G0can be observed only in the energy interval from approximately 1 to 7 eV hence for energies above the Fermi level. Once again, this follows our previous observations for the transmission results for the Π states concluded from Figure 6. Nonetheless, only on the basis of the results presented in Figure 7 can we note that due to the summation over all possible state contributions which constitute the G(E) spectra, not only the σ∗-state electrons, but also some of those in the degenerate Π states contribute to the high conductance values in the cited energy intervals. This important observation proves that the σ∗- and Π-state electrons are of crucial importance for both the zero-bias quantum conductance of the silicon-doped carbon wires and the possible finite bias ones. This implies that the use of only a single orbital for the description of the carbon atoms will result in an inadequate description of the transport processes across low-coordinated systems containing these atoms.
In the present work, the unknown properties of the quantum electronic conductance for nanojunctions made of silicon-doped carbon wires between carbon leads are studied in depth. This is done using the phase field matching theory and the tight-binding method. The local basis for the electronic wave functions is assumed to be composed of four different atomic orbitals for silicon and carbon, namely the s, p x , p y , and p z states.
In the first step, we calculate the electronic band structures for three nanomaterials, namely the one-dimensional infinite wires of silicon, carbon, and diatomic silicon carbide. This permits a matching comparison with the available corresponding DFT results, with the objective to select the optimal TB parameters for the three nanomaterials.
This optimal set of the tight-binding parameters is then used to calculate the electronic conductance across the silicon-doped carbon wire nanojunctions. Five different nanojunction cases are analyzed to sample their behavior under different atomic configurations. We show that despite the nonconducting character of the infinite silicon carbide wires, its finite implementation as nanojunctions exhibit a finite conductance. This outcome is explained by the energy difference between the binding energies of the silicon and carbon atoms, which correspond to an effective potential barrier for the degenerate Π-state electrons transmitted across the nanojunction under zero-bias field.
The conductance effects that may arise due to minimal substitutional disorder and to artificially organize symmetry considerations on the silicon carbide wire nanojunction are also investigated. By exchanging the positions of two silicon and carbon atoms on an initial nanojunction to generate a substitutional disorder, we show that the total quantum conductance is suppressed at the Fermi level. This is in sharp contrast with the finite and significant conductance for the initial atomically ordered nanojunction with periodic configurations of the silicon and carbon atoms. Also, the analysis of a silicon carbide nanojunction of a comparable size as the one above, presenting symmetry properties, shows that quantum conductance is suppressed at the Fermi level.
In summary, we note that the biggest maxima of the conductance spectra for the zero-bias limit can be observed for high energies for all of the considered systems. This conclusion reveals the fact that electrons incident from the leads in both σ∗and Π states are crucial for the considerations of the electronic transport properties of the silicon-doped carbon wire nanojunctions.
Explicit forms of the Ei,jand Hi,jmatrices
The explicit forms of the submatrices of Equation 1 are given in the following manner:
Equations 22 and 23 denote N x N l square matrices, where matrix (Equation 23) is upper triangular. In this manner, component matrices (Equations 24 and 25) are of the dimension N l ×N l . Additionally, matrix always denotes diagonal matrix, while matrix is much more complex, with possible nonzero elements at every position. Please note that some of the elements can vanish due to symmetry conditions and simplify the notation of the matrix.
The partitioning technique is a suitable method which allows to avoid the singularity problem of the HN,N−1 and matrices and calculates only nontrivial solutions of Equation 10. Detailed discussion of the partitioning technique is presented in the work of Khomyakov and Brocks , and this section gives only our short remarks on this method.
In Equation 27, parameter N n stands for the order of nearest-neighbor interactions assumed in calculations, e.g., N n =1 for the first nearest-neighbor interactions. On the basis of Equations 26 and 27, the reduced 2N l eigenvalue problem is written as follows:
Please note that the reduced problem of Equation 28 gives 2N l eigenvalues with 2N l corresponding eigenvectors; this N x times less than can be expected from a physical point of view. Nevertheless, those solutions can be easily separated into N x N l eigenvalues and N x N l eigenvectors of a purely physical character.
Explicit forms of the Mi,j, , and components
The submatrices of the matched(D + 2)×(D + 2) square matrix M in Equation 16, for a given i and j indices, are given as follows:
except for the submatrices which describe the boundary atoms of the system and those that are expressed in the following manner:
Finally, the and of Equation 16 vector components are written as follows:
As specified in the ‘Phase field matching theory’ subsection, the group velocities for individual states can be calculated on the basis of Equation 6 rewritten in the following manner:
where v denotes the eigenvalues of Equation 39 which yields all required electron group velocities for each propagating state. Further, V is the N x ×N l size matrix of the following form:
Finally, v(R N ,k) stands for eigenvectors of the problem of Equation 39. We note that, usually, Equation 40 includes the constant part d β /h, where h is the Planck constant. However, for the purpose of electronic conductance calculations within the PFMT approach, this term can be omitted due to the fact that only the ratios of the given group velocities are important (please see Equations 17 and 18).
Agraït N, Levy-Yeyati A, van Ruitenbeek JM: Quantum properties of atomic-sized conductors. Phys Rep 2003, 377: 81–279. 10.1016/S0370-1573(02)00633-6
Nitzan A, Ratner M: Electron transport in molecular wire junctions. Science 2003, 300: 1384–1389. 10.1126/science.1081572
Wan CC, Mozos JL, Taraschi G, Wang J, Guo H: Quantum transport through atomic wires. Appl Phys Lett 1997, 71: 419–421. 10.1063/1.119328
Geim AK, Novoselov KS: The rise of graphene. Nature Mater 2007, 6: 183–191.
Kroto HW, Heath JR, O’Brien SC, Curl RF, Smalley RE: C60: buckminsterfullerene. Nature 1985, 318: 162–163. 10.1038/318162a0
Iijima S, Ichihashi T: Single-shell carbon nanotubes of 1-nm diameter. Nature 1993, 363: 603–605. 10.1038/363603a0
Euen PL: Nanotechnology: carbon-based electronics. Nature 1998, 393: 15–16. 10.1038/29874
Heath JR, Zhang Q, O’Brien SC, Curl RF, Kroto HW, Smalley RE: The formation of long carbon chain molecules during laser vaporization of graphite. J Am Chem Soc 1987, 109: 359–363. 10.1021/ja00236a012
Lagow RJ, Kampa JJ, Wei HC, Battle SL, Genge JW, Laude DA, Harper CJ, Bau R, Stevens RC, Haw JF, Munson E: Synthesis of linear acetylenic carbon: the “sp” carbon allotrope. Science 1995, 267: 362–367. 10.1126/science.267.5196.362
Derycke V, Soukiassian P, Mayne A, Dujardin D, Gautier J: Carbon atomic chain formation on the β-SiC(100) surface by controlled sp→sp3 transformation. Phys Rev Lett 1998, 81: 5868–5871. 10.1103/PhysRevLett.81.5868
Troiani HE, Miki-Yoshida M, Camacho-Bragado GA, Marques MAL, Rubio A, Ascencio JA, Jose-Yacaman M: Direct observation of the mechanical properties of single-walled carbon nanotubes and their junctions at the atomic level. Nano Lett 2003, 3: 751–755. 10.1021/nl0341640
Zhao X, Ando Y, Liu Y, Jinno M, Suzuki T: Carbon nanowire made of a long linear carbon chain inserted inside a multiwalled carbon nanotube. Phys Rev Lett 2003, 90: 187401.
Yuzvinsky TD, Mickelson W, Aloni S, Begtrup GE, Kis A, Zettl A: Shrinking a carbon nanotube. Nano Lett 2006, 6: 2718–2722. 10.1021/nl061671j
Jin C, Lan H, Peng L, Suenaga K, Iijima S: Deriving carbon atomic chains from graphene. Phys Rev Lett 2009, 102: 205501.
Kértesz M, Koller J, Az̆man A: Ab initio Hartree-Fock crystal orbital studies. II. Energy bands of an infinite carbon chain. J Chem Phys 1978, 68: 2779–2782. 10.1063/1.436070
Kértesz M, Koller J, Az̆man A: Different orbitals for different spins for solids: fully variational ab initio studies on hydrogen and carbon atomic chains, polyene, and poly(sulphur nitride). Phys Rev B 1979, 19: 2034–2040. 10.1103/PhysRevB.19.2034
Karpfen A: Ab initio studies on polymers. I. The linear infinite polyyne. J Phys C Solid State Phys 1979, 12: 3227–3237. 10.1088/0022-3719/12/16/011
Teramae M, Yamabe T, Imamura A: Ab initio effective core potential studies on polymers. Theor Chim Acta 1983, 64: 1–12.
Springborg M: Self-consistent, first principles calculations of the electronic structures of a linear, infinite carbon chain. J Phys C 1986, 19: 4473–4482. 10.1088/0022-3719/19/23/010
Rice MJ, Phillpot SR, Bishop AR, Campbell DK: Solitons, polarons, and phonons in the infinite polyyne chain. Phys Rev B 1986, 34: 4139–4149. 10.1103/PhysRevB.34.4139
Springborg M, Dreschel SL, Málek J: Anharmonic model for polyyne. Phys Rev B 1990, 41: 11954–11966. 10.1103/PhysRevB.41.11954
Watts JD, Bartlett RJ: A theoretical study of linear carbon cluster monoanions, Cn− and dianions, Cn2− (n=2−10). J Chem Phys 1992, 97: 3445–3457. 10.1063/1.462980
Xu CH, Wang CZ, Chan CT, Ho KM: A transferable tight-binding potential for carbon. J Phys Condens Matter 1992, 4: 6047–6054. 10.1088/0953-8984/4/28/006
Lou L, Nordlander P: Carbon atomic chains in strong electric fields. Phys Rev B 1996, 54: 16659–16662. 10.1103/PhysRevB.54.16659
Jones RO, Seifert G: Density functional study of carbon clusters and their ions. Phys Rev Lett 1997, 79: 443–446. 10.1103/PhysRevLett.79.443
Fuentealba P: Static dipole polarizabilities of small neutral carbon clusters Cn (n ⩽ 8). Phys Rev A 1998, 58: 4232–4234. 10.1103/PhysRevA.58.4232
Abdurahman A, Shukla A, Dolg M: Ab initio many-body calculations of static dipole polarizabilities of linear carbon chains and chainlike boron clusters. Phys Rev B 2002, 65: 115106.
Cahangirov S, Topsakal M, Ciraci S: Long-range interactions in carbon atomic chains. Phys Rev B 2010, 82: 195444.
Tongay S, Ciraci S: Atomic strings of group IV, III-V, and II-VI elements. Appl Phys Lett 2004, 85: 6179–6181. 10.1063/1.1839647
Bylaska EJ, Weare JH, Kawai R: Development of bond-length alternation in very large carbon rings: LDA pseudopotential results. Phys Rev B 1998, 58: R7488—R7491.
Zhang Y, Su Y, Wang L, Kong ESW, Chen X, Zhang Y: A one-dimensional extremely covalent material: monatomic carbon linear chain. Nanoscale Res Lett 2011, 6: 577. 10.1186/1556-276X-6-577
Lang ND, Avouris P: Oscillatory conductance of carbon-atom wires. Phys Rev Lett 1998, 81: 3515–3518. 10.1103/PhysRevLett.81.3515
Lang ND, Avouris P: Carbon-atom wires: charge-transfer doping, voltage drop, and the effect of distortions. Phys Rev Lett 2000, 84: 358–361. 10.1103/PhysRevLett.84.358
Larade B, Taylor J, Mehrez H, Guo H: Conductance, I-V curves, and negative differential resistance of carbon atomic wires. Phys Rev B 2001, 64: 075420.
Tongay S, Dag S, Durgun E, Senger RT, Ciraci S: Atomic and electronic structure of carbon strings. J Phys Cond Matter 2005, 17: 3823–3836. 10.1088/0953-8984/17/25/009
Senger RT, Tongay S, Durgun E, Ciraci S: Atomic chains of group-IV elements and III-V and II-VI binary compounds studied by a first-principles pseudopotential method. Phys Rev B 2005, 72: 075419.
Baranović G, Z̆ Crljen: Unusual conductance of polyyne-based molecular wires. Phys Rev Lett 2007, 98: 116801.
Okano S, Tománek D: Effect of electron and hole doping on the structure of, C, Si, and S nanowires. Phys Rev B 2007, 75: 195409.
Chen W, Andreev AV, Bertsch GF: Conductance of a single-atom carbon chain with graphene leads. Phys Rev B 2009, 80: 085410.
Wang Y, Lin ZZ, Zhang W, Zhuang J, Ning XJ: Pulling long linear atomic chains from graphene: molecular dynamics simulations. Phys Rev B 2009, 80: 233403.
Song B, Sanvito S, Fang H: Anomalous I-V curve for mono-atomic carbon chains. New J Phys 2010, 12: 103017. 10.1088/1367-2630/12/10/103017
Zhang GP, Fang XW, Yao YX, Wang CZ, Ding ZJ, Ho KM: Electronic structure and transport of a carbon chain between graphene nanoribbon leads. J Phys Cond Matter 2011, 23: 025302. 10.1088/0953-8984/23/2/025302
Ke Y, Xia K, Guo H: Disorder scattering in magnetic tunnel junctions: theory of nonequilibrium vertex correction. Phys Rev Lett 2008, 100: 166805.
Nozaki D, Pastawski HM, Cuniberti G: Controlling the conductance of molecular wires by defect engineering. New J Phys 2010, 12: 063004. 10.1088/1367-2630/12/6/063004
Strupiński W, Grodecki K, Wysmołek A, Stȩpniewski R, Szkopek T, Gaskell PE, Grüneis A, Haberer D, BoŻek R, Krupka J, Baranowski JM: Graphene epitaxy by chemical vapor deposition on SiC. Nano Lett 2011, 11: 1786–1791. 10.1021/nl200390e
Wang F, Shepperd K, Hicks J, Nevius MS, Tinkey H, Tejeda A, Taleb-Ibrahimi A, Bertran F, Fèvre PL, Torrance DB, First PN, de Heer WA, Zakharov AA, Conrad EH: Silicon intercalation into the graphene-SiC interface. Phys Rev B 2012, 85: 165449.
Landauer R: Spatial variation of currents and fields due to localized scatterers in metallic conduction. IBM J Res Dev 1957, 1: 223–231.
Büttiker M: Four-terminal phase-coherent conductance. Phys Rev Lett 1986, 57: 1761–1764. 10.1103/PhysRevLett.57.1761
Zwierzycki M, Xia K, Kelly PJ, Bauer GEW, Turek I: Spin injection through an Fe/InAs interface. Phys Rev B 2003, 67: 092401.
Pauly F, Viljas JK, Huniar U, Häfner M, Wohlthat S, Bürkle M, Cuevas JC, Schön G: Cluster-based density-functional approach to quantum transport through molecular and atomic contacts. New J Phys 2008, 10: 125019. 10.1088/1367-2630/10/12/125019
Caroli C, Combescot R, Nozières P, Saint-James D: Direct calculation of the tunneling currents. J Phys C 1971, 8: 916–929.
Deretzis I, Magna AL: Coherent electron transport in quasi one-dimensional carbon-based systems. Eur Phys J B 2011, 81: 15. 10.1140/epjb/e2011-20134-x
Khater A, Szczȩśniak D: A simple analytical model for electronic conductance in a one dimensional atomic chain across a defect. J Phys Conf Ser 2011, 289: 012013.
Szczȩśniak D, Khater A: Electronic conductance via atomic wires: a phase field matching theory approach. Eur Phys J B 2012, 85: 174.
Khater A, Bourahla B, Abou Ghantous M, Tigrine R, Chadli R: Magnons coherent transmission and heat transport at ultrathin insulating ferromagnetic nanojunctions. Eur Phys J B 2011, 82: 53–61. 10.1140/epjb/e2011-10935-2
Khater A, Belhadi M, Abou Ghantous M: Phonons heat transport at an atomic well boundary in ultrathin solid films. Eur Phys J B 2011, 80: 363–369. 10.1140/epjb/e2011-10892-8
Tigrine R, Khater A, Bourahla B, Abou Ghantous M, Rafli O: Magnon scattering by a symmetric atomic well in free standing very thin magnetic films. Eur Phys J B 2008, 62: 59–64. 10.1140/epjb/e2008-00125-x
Virlouvet A, Khater A, Aouchiche H, Rafli O, Maschke K: Scattering of vibrational waves in perturbed two-dimensional multichannel asymmetric waveguides as on an isolated step. Phys Rev B 1999, 59: 4933–4942. 10.1103/PhysRevB.59.4933
Fellay A, Gagel F, Maschke K, Virlouvet A, Khater A: Scattering of vibrational waves in perturbed quasi-one-dimensional multichannel waveguides. Phys Rev B 1997, 55: 1707–1717. 10.1103/PhysRevB.55.1707
Mardaani M, Rabani H, Esmaeili A: An analytical study on electronic density of states and conductance of typical nanowires. Solid State Commun 2011, 151: 928–932. 10.1016/j.ssc.2011.04.010
Rabani H, Mardaani M: Exact analytical results on electronic transport of conjugated polymer junctions: renormalization method. Solid State Commun 2012, 152: 235–239. 10.1016/j.ssc.2011.09.026
Wu Y, Childs PA: Conductance of graphene nanoribbon junctions and the tight binding model. Nanoscale Res Lett 2011, 6: 62.
Chen J, Yang L, Yang H, Dong J: Electronic and transport properties of a carbon-atom chain in the core of semiconducting carbon nanotubes. Phys Lett A 2003, 316: 101–106. 10.1016/S0375-9601(03)01132-0
Hands ID, Dunn JL, Bates CA: Visualization of static Jahn-Teller effects in the fullerene anion C60−. Phys Rev B 2010, 82: 155425.
Delga A, Lagoute J, Repain V, Chacon C, Girard Y, Marathe M, Narasimhan S, Rousset S: Electronic properties of Fe clusters on a Au(111) surface. Phys Rev B 2011, 84: 035416.
Slater JC, Koster GF: Simplified LCAO method for the periodic potential problem. Phys Rev 1954, 94: 1498–1524. 10.1103/PhysRev.94.1498
Harrison WA: Elementary Electronic Structure. Singapore: World Scientific; 2004.
Zhang L, Wang JS, Li B: Ballistic magnetothermal transport in a Heisenberg spin chain at low temperatures. Phys Rev B 2008, 78: 144416.
Bekaroglu E, Topsakal M, Cahangirov S, Ciraci S: First-principles study of defects and adatoms in silicon carbide honeycomb structures. Phys Rev B 2010, 81: 075433.
Kaxiras E: Atomic and Electronic Structure of Solid. New York: Cambridge University Press; 2003.
Khomyakov PA, Brocks G: Real-space finite-difference method for conductance calculations. Phys Rev B 2004, 70: 195402.
D Szczȩśniak would like to thank the French Ministry of Foreign Affairs for his PhD scholarship grant CNOUS 2009-2374, to the Polish National Science Center for their research grant DEC-2011/01/N/ST3/04492, and to the Graduate School of Sciences at the University du Maine for their support.
The authors declare that they have no competing interests.
DS participated in the design of this study, in analytical calculations, and in writing the code for numerical calculations, carried out numerical calculations, drafted the manuscript, and participated in writing the final version of the manuscript. AK coordinated this study, participated in its design and analytical calculations, and in writing the final version of the manuscript. ZB participated in the design of this study, its coordination, and substantial critical revision of the final version of the manuscript. RS participated in writing the code for numerical calculations and substantial critical revision of the final version of the manuscript. MAG participated in the substantial critical revision of the final version of the manuscript. All authors read and approved the final manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
About this article
Cite this article
Szczȩśniak, D., Khater, A., Ba̧k, Z. et al. Quantum conductance of silicon-doped carbon wire nanojunctions. Nanoscale Res Lett 7, 616 (2012). https://doi.org/10.1186/1556-276X-7-616
- Quantum wires
- Electronic transport
- Finite-difference methods